Probe effect in scanning tunneling microscopy on Si 001 ... Probe effect in scanning tunneling...
Embed Size (px)
Transcript of Probe effect in scanning tunneling microscopy on Si 001 ... Probe effect in scanning tunneling...
Probe effect in scanning tunneling microscopy on Si„001… low-temperature phases
Shoji Yoshida,1 Tomohiko Kimura,1 Osamu Takeuchi,1 Kenji Hata,1,* Haruhiro Oigawa,1 Toshihiko Nagamura,2
Hiroshi Sakama,3 and Hidemi Shigekawa1,† 1Institute of Applied Physics, 21st Century COE, NANO project, CREST, University of Tsukuba, Tsukuba 305-8573, Japan
2Unisoku Co. Ltd., Hirakata, Osaka 573-0131, Japan 3Department of Physics, Sophia University, Tokyo 102-8554, Japan
(Received 18 February 2004; published 9 December 2004)
The probe effect, the effect of parameters in scanning tunneling microscopy(STM) measurement, on the Sis100d surface with two competing phases in delicate balance, was investigated systematically by reexamining its influence on the Sis100d dimer flip-flop motions at 5 and 80 K. On the basis of the results, the complex array of the phenomena of the Sis100d surface structures was comprehended. The phase transition between cs432d andps232d structures below,40 K was studied by STM, as well as by low-energy electron diffrac- tion, and the appearance of theps232d structure at a reduced probe effect was confirmed. In these investiga- tions, a phase with long-range ordering of thecs432d andps232d structures was observed.
DOI: 10.1103/PhysRevB.70.235411 PACS number(s): 68.35.Rh, 61.14.Hg, 68.35.Bs, 68.37.Ef
All experimental measurements inevitably influence the results obtained. Scanning tunneling microscopy(STM) is a very powerful method for the analyses of physical and chemical phenomena because of its high potential to probe the local electronic structures of materials. However, as has been pointed out, STM parameters, such as bias voltage, tun- neling current, and tip-sample distance, influence the sample characteristics.1–8 For example, as was recently clarified in the photovoltage measurement, tunneling of a small amount of the photoexcited carriers influences the local band bend- ing and results in the scattering of the results depending on the measurement conditions.1,2 Inelastic-tunneling spectros- copy is one of the promising techniques included in STM, and when the bias voltage is adjusted to the selected vibra- tional mode, even chemical reactions can be induced at less than a few volts.3,4 This effect may critically influence the results obtained.
These effects have generally not been taken into account, when the surface structures of semiconductors and metals are the target, because of their stable structures under ordinary experimental measurement conditions. However, recently, STM analysis of the Sis100d surface has been recognized as one of the cases in which the effect of the experimental pro- cesses is apparent.5–8 Namely, despite its great importance, the ground state of the Sis100d surface is still one of the most controversial issues in surface science. Since the Sis100d sur- face has two competing phases in delicate balance, the per- turbations by STM measurement are considered to play an essential role in the chaotic situation.
On the Sis100d surface, pairs of top-layer atoms form dimers, which gives rise to as231d structure;9,10 however, the s231d phase is not the Sis100d ground state, and differ- ent reconstructions within similar dimer structures are pos- sible. The energetically favored alternation of dimer buckling along the dimer rows leads to the two phases. One is the cs432d reconstruction, in which alternating buckling angles are also present between two neighboring dimer rows. An-
other possible phase is theps232d phase, in which the buck- ling angle is the same between two neighboring dimer rows. The difference between the energies of theps232d and cs432d reconstructions obtained by theoretical calculations is only of the order of 1 meV per dimer,10 which further complicates the issue.
From low-energy electron diffraction(LEED) measure- ments, the reversible second-order phase transition between the disordereds231d and orderedcs432d phases is found to occur at,200 K.11–13 The most stable phase was con- cluded to be thecs432d phase. Through low-temperature STM studies at,140 K, thecs432d structure was also con- firmed to be the most stable arrangement of the buckled dimers.14,15 The s231d phase observed by STM at room temperature was attributed to the quick flip-flop motion of the buckled dimers.16,17These results seemed to have settled the controversy; however, in subsequent intensive studies on the low-temperature phase of Sis100d by STM and atomic force microscopy,cs432d, ps232d /cs432d (coexisting), and symmetric dimer phases were observed to exist below 40 K, which gave rise to further controversy regarding the ground state of Sis100d.6–8,18–25
Recently, in order to solve this issue, STM measurement conditions, such as the effect of the external electric field and tunneling current, were reconsidered.5–8,26–29In addition, the surface was studied by LEED to reduce the probe effect.31
However, theps232d, cs432d, and disordered phases with buckled dimers were identified again for the respective cases.6,7,30
These results indicate that there still exists a controversy regarding the ground state, which, however, is due to the difficulty in comprehending the essential point of a complex array of the phenomena. For example, thecs432d phase, the dominantly observed structure by STM at low bias voltage, changed into theps232d phase with increasing bias voltage. Similar structural change, fromcs432d to ps232d, was also observed upon decreasing the tunneling current with the bias voltage held constant. With the latter case left unexplained, thecs432d phase was concluded to be the ground state, and
PHYSICAL REVIEW B 70, 235411(2004)
1098-0121/2004/70(23)/235411(11)/$22.50 ©2004 The American Physical Society235411-1
the appearance of theps232d phase was considered as a bias-voltage-induced artificial structure.7 However, when the two results are taken into consideration together, the ps232d phase appears when the tip-sample distance is in- creased, namely, under the condition of a reduced probe ef- fect. Even for the LEED measurement, the effect of the probe electrons has been pointed out.31 Therefore, it is im- portant to analyze the phenomena systematically to gain comprehensive understanding.
In this paper we present our results of the reexamination of the STM probe effect, the key issue that has been causing the current controversy. Systematic study of the Si dimer flip-flop motion proved the existence of the probe effect in STM measurement both at 80 and 5 K and the appearance of theps232d phase under a reduced probe effect condition. In these investigations, a phase with a long-range ordering of the cs432d andps232d structures was observed.
After prebaking for,5 h at ,700 °C under a vacuum pressure below 5.0310−9 Pa, the Sis100d samples(P and As doped: 0.01–0.001V) were heated at 1200 °C for 10 s. Af- ter the samples were cooled to 5 K, an additional flash heat- ing was carried out to reduce the defect density and the effect of the adsorbates. Sample temperature was measured with a thermocouple or a Si-diode sensor attached to the sample holder.
III. RESULTS AND DISCUSSIONS
In order to understand the STM probe effect comprehen- sively, its influence on the dimer flip-flop motion was ana- lyzed systematically. First, the flip-flop motion induced at high bias voltage was examined. Next, the probe effect at low bias voltage was examined by observing the dynamics of P defects. The details will be described later. Then, the phase transition betweencs432d and ps232d structures below ,40 K was studied by LEED as well as by STM. Thereby, the appearance of theps232d structure at a reduced probe effect was confirmed well. Through these investigations, a phase with a long-range ordering of thecs432d and ps2 32d structures was observed.
A. Analysis of the STM probe effect
1. Inelastic tunneling in high-bias-voltage region at 5 K
Figures 1(a)–1(f) show the STM images obtained in the constant current mode at the same area with six different bias voltages. Symmetric and buckled dimers were imaged at high [(a) and (d)] and lower[(c) and (f)] bias voltages, re- spectively. These characteristics are in good agreement with those reported in other papers.6–8 However, the noteworthy point is that, in the middle-bias range(−0.95 V and 1.45 V), the image of the dimers is rather noisy compared to those at higher bias voltages. The difference is clearer in the line profiles shown in Fig. 1(g), which were taken along the white lines in Figs. 1(a) and 1(b).
To examine this point further, the tunneling current was measured with the STM tip being held above a Si dimer with a weak feedback.32 As shown in Fig. 1(h), the tunneling cur- rent changes between two well-defined values, indicating the flip-flop motion of the dimer[Fig. 2(a)], as was observed in the previous studies.32
These characteristics are similar to the change in the temperature-dependent dimer images between 80 K and room temperature(RT), as was described in the Introduction. Namely, the symmetric dimers at high-bias voltage are con- sidered to be caused by the averaged image of the fast flip- flopping motion of dimers, instead of the stable symmetric one.
In order to clarify the probe effect on the flip-flop motion, the bias dependence of the flip-flop rate was observed with the current held constant at 0.2 nA. For the flip-flop rate shown in Fig. 2(b) as a function of the bias voltage, we find thresholds(,−0.90 V and,+1.45 Vd for the process. On the other hand, the flip-flop rate increased with increasing tunneling current, as shown in Fig. 2(c). Here bias voltage was held at −0.90 V, just above the threshold, to measure